FZ/T 73027-2016 English PDF (FZT73027-2016)
FZ/T 73027-2016 English PDF (FZT73027-2016)
FZ/T 73027-2016: Knitted warp lace
TEXTILE INDUSTRY STANDARD
Replacing FZ/T 73027-2008
Knitted warp lace
ISSUED ON. OCTOBER 22, 2016
IMPLEMENTED ON. APRIL 01, 2017
Issued by. Ministry of Industry and Information Technology of the People's Republic of China
Table of Contents
1 Scope... 5
2 Normative references... 5
3 Terms and definitions... 6
4 Product classification... 7
5 Specifications... 7
6 Requirements... 7
7 Testing... 12
8 Determination rules... 16
9 Marking, packaging, transportation and storage... 16
10 Others... 16
Knitted warp lace
This Standard specifies the terms and definitions, product classification, specifications, requirements, tests, judgment rules, marking, packaging, transportation and storage of knitted warp lace.
This Standard applies to the assessment of the quality of knitted warp lace finished products.
2 Normative references
The following referenced documents are indispensable for the application of this document. For dated references, only the edition cited applies to this document. For undated references, the latest edition (including any amendment) applies to this document.
GB/T 250, Textiles - Tests for colour fastness - Grey scale for assessing change in colour
GB/T 2910, Textiles - Quantitative chemical analysis
GB/T 2912.1, Textiles - Determination of formaldehyde - Part 1.Free and hydrolyzed formaldehyde (water extraction method)
GB/T 3920, Textiles - Tests for colour fastness - Colour fastness to rubbing GB/T 3921-2008, Textiles - Tests for colour fastness - Colour fastness to washing with soap or soap and soda
GB/T 3922, Textiles - Tests for colour fastness - Colour fastness to perspiration GB/T 4856, Package of cotton goods and knitwear
GB 5296.4, Instructions for use of products of consumer interest - Part 4.Textiles and apparel
GB/T 5713, Textiles - Tests for colour fastness - Colour fastness to water GB/T 7573, Textiles - Determination of pH of aqueous extract
GB/T 8170, Rules of rounding off for numerical values and expression and judgment of limiting values
GB/T 8427-2008, Textiles - Tests for color fastness - Color fastness to artificial light. Xenon arc fading lamp test
GB/T 8628, Textiles - Preparation, marking and measuring of fabric specimens and garments in tests for determination of dimensional change
GB/T 8629, Textiles - Domestic washing and drying procedures for textile testing GB/T 8630, Textiles - Determination of dimensional change in washing and drying GB/T 14801, Test method for skewness and bow in woven and knitted fabrics GB/T 17592, Textiles - Determination of the banned azo colourants
GB 18401, National general safety technical code for textile products
GB/T 29862, Textiles - Identification of fiber content
GB 31701, Safety technical code for infants and children textile products FZ/T 01026, Textiles - Quantitative chemical analysis - Multi-component fibre mixtures
FZ/T 01057 (all parts), Test method for identification of textile fibres FZ/T 01095, Textile - Test method of elastane fibre content
FZ/T 70006, Stretch and recovery testing method for knits
FZ/T 70010, Testing method of dry weight per unit area for knitted fabrics 3 Terms and definitions
The following terms and definitions are applicable to this document.
3.1 Pattern length
The distance of a complete loop pattern along the knitting direction of knitted warp lace. 3.2 Pattern width
The distance between the parallel lines of the widest point on both sides of the pattern, when the knitted warp lace is perpendicular to the lace knitting direction. 4 Product classification
4.1 Knitted warp lace is divided into elastic knitted warp lace and non-elastic knitted warp lace by whether the fabric bottom net contains elastic fibers.
4.2 Knitted warp lace is divided into lace and lace fabric by pattern width, where the width is less than 80 cm, it is lace, and where the width is greater than or equal to 80 cm, it is lace fabric.
The specifications of knitted warp lace are expressed as. breadth × pattern length × pattern width × dry weight per square meter (or dry weight per unit length); elastic lace also needs to be marked with tensile elastic elongation. Among them, the breadth, pattern length and pattern width are expressed in cm, the dry weight per square meter (or dry weight per unit length) is expressed in g/m2 (or g/m), and the tensile elastic elongation is expressed in %.
6.1 Contents of requirements
The requirements for knitted warp lace are divided into two aspects. inherent quality and appearance quality. Inherent quality includes fiber content, dry weight deviation rate, washing size change rate, loose edge after washing, tensile elastic elongation, color fastness to washing with soap or soap and soda, color fastness to perspiration, color fastness to water, color fastness to rubbing, color fastness to light, formaldehyde content, pH value, resoluble carcinogenic aromatic amine dyes, unpleasant odor and other indicators; appearance quality is divided into size deviation rate, same roll (or piece) color difference, same batch color difference, straying end, local defects and scattered defects and other indicators.
6.2 Gradation requirements
6.2.1 Knitted warp lace is divided into high-quality products, first-class products and qualified products.
6.2.2 The inherent quality is rated by batches, and the appearance quality is rated by rolls (or pieces). The combination of the two is graded at the lowest grade. 6.2.3 For each indicator of inherent quality, the lowest inspection result shall be used as the evaluation basis for this batch of products.
6.4.4 For local defects, grading shall be carried out according to the range specified in Table 3 and Table 4, and each grading shall be 10 cm.
6.4.5 When measuring the appearance defects, measure by the maximum length. 6.4.6 Slitting defects. 1 defect is counted for each occurrence of rotten edge, burr, uneven teeth, etc.
6.4.7 Trimming thread end. the length shall be within 0.3 cm, otherwise, 1 defect shall be counted.
6.4.8 Holes. Where there are several holes within 3 cm of the lace fabric at the same time, it shall be counted as one. The dropped stitch and bad stitch, within 10 cm, caused by the holes will not be counted; otherwise, it shall be regarded as a dropped stitch or bad stitch.
7.1 Inherent quality
7.1.1 Specimen preparation
188.8.131.52 Randomly take samples according to the type, specification and color of the delivery batch. The number of samples shall be sufficient for all tests (including 3 pieces of 700 mm full-breadth samples for the washing size change rate).
184.108.40.206 The sampling distance shall be at least 1.5 m from the cloth head, and the samples taken shall not have defects that affect the test results.
7.1.2 Test method
220.127.116.11 Fiber content
Carry out according to GB/T 2910 (all parts), FZ/T 01026, FZ/T 01057 (all parts), FZ/T 01095 and other regulations.
18.104.22.168 Dry weight deviation rate
22.214.171.124.1 The dry weight per square meter shall be tested in accordance with the provisions of FZ/T 70010.For the test of dry weight per unit length, according to the entire breadth of the lace, take 3 pieces evenly according to one or several complete patterns along the length direction, measure the length, dry and weigh, and calculate the dry weight per unit length. For the dry weight per square meter of lace fabric with uneven structure, take samples by the method of the test of dry weight per unit length, measure the length and width of the sample, dry and weigh it, and calculate its dry weight per square meter.
Perform according to GB/T 5713.
126.96.36.199 Color fastness to light
Perform according to Method 3 of GB/T 8427-2008.
188.8.131.52 Formaldehyde content
Perform according to GB/T 2912.1.
184.108.40.206 pH value
Perform according to GB/T 7573.
220.127.116.11 Resoluble carcinogenic aromatic amine dyes
Perform according to GB/T 17592.
18.104.22.168 Unpleasant odor
Perform according to GB 18401.
7.2 Appearance quality
7.2.1 Detection rules
22.214.171.124 Visual inspection shall be adopted as the inspection method of appearance quality.
126.96.36.199 The appearance quality shall be randomly sampled by variety, specification and color according to the delivery batch number, and the sampling quantity shall not be less than 2%, but not less than 2 rolls (or pieces).
7.2.2 Inspection conditions
Appearance quality inspection is mainly based on the front of the product, by cloth inspecting machine inspection or on a horizontal inspection table, using normal daytime northern light or fluorescent lighting; the illumination is not less than 750 lx, and the distance between the eyes and the cloth surface is about 60 cm. The speed of the cloth inspecting machine is 16 m/min ~ 18 m/min.
188.8.131.52 Size deviation rate
184.108.40.206.1 Tools. steel ruler or steel tape, the length of which must be greater than the width of the sample, and the accuracy is 0.1 cm.